# Strain Effect on Electronic Structure and Work Function in ... › 0045 › 168f0eb4bb6......

date post

06-Jul-2020Category

## Documents

view

1download

0

Embed Size (px)

### Transcript of Strain Effect on Electronic Structure and Work Function in ... › 0045 › 168f0eb4bb6......

materials

Article

Strain Effect on Electronic Structure and Work Function in α-Fe2O3 Films

Li Chen 1,*, Changmin Shi 1, Xiaolong Li 1, Zhishan Mi 2, Dongchao Wang 1, Hongmei Liu 1

and Lijie Qiao 2,* 1 Institute of Condensed Matter Physics, Linyi University, Linyi 276000, China;

[email protected]n (C.S.); [email protected] (X.L.); [email protected] (D.W.); [email protected] (H.L.)

2 Corrosion and Protection Center, Key Laboratory for Environmental Fracture (MOE), University of Science and Technology Beijing, Beijing 100083, China; [email protected]

* Correspondence: [email protected] (L.C.); [email protected] (L.Q.); Tel.: +86-539-8766236 (L.C.)

Academic Editor: Alex A. Volinsky Received: 14 January 2017; Accepted: 6 March 2017; Published: 9 March 2017

Abstract: We investigate the electronic structure and work function modulation of α-Fe2O3 films by strain based on the density functional method. We find that the band gap of clean α-Fe2O3 films is a function of the strain and is influenced significantly by the element termination on the surface. The px and py orbitals keep close to Fermi level and account for a pronounced narrowing band gap under compressive strain, while unoccupied dz2 orbitals from conduction band minimum draw nearer to Fermi level and are responsible for the pronounced narrowing band gap under tensile strain. The spin polarized surface state, arising from localized dangling-bond states, is insensitive to strain, while the bulk band, especially for pz orbital, arising from extended Bloch states, is very sensitive to strain, which plays an important role for work function decreasing (increasing) under compressive (tensile) strain in Fe termination films. In particular, the work function in O terminated films is insensitive to strain because pz orbitals are less sensitive to strain than that of Fe termination films. Our findings confirm that the strain is an effective means to manipulate electronic structures and corrosion potential.

Keywords: α-Fe2O3 films; strain; band gap; work function; corrosion potential

PACS: 71.20.Nr; 71.70.Fk; 73.20.At

1. Introduction

Metals are protected from corrosion in many aqueous environments by the formation of “passive” oxide films that are typically only a few nanometers thick. The transition metal oxides are an important class of functional materials [1] because of their localized d electrons [2–4]. Among the iron oxides, α-Fe2O3, hematite, with an experimental band gap of 2.2 eV [5] was identified as a charge transfer semiconductor [2] rather than a Mott–Hubbard insulator because the upper edge of the valence band is dominated by oxygen p states. Below the Néel temperature (955 K), α-Fe2O3 is an antiferromagnetic (AFM) insulator showing weak ferromagnetism above the Morin temperature (260 K), due to a slight canting of the two sublattice magnetizations [6]. The geometric, electronic, and magnetic properties [7–9]; carrier effective masses [10]; and other related properties on Fe2O3 [11] were present in theoretical work.

The technological importance of these films has led to widespread investigation of their structure, chemistry [12] and practical applications such as water splitting [13]. The atomic structure of α-Fe2O3 is important to passivity, since this often controls its protective properties, where interfacial strain due

Materials 2017, 10, 273; doi:10.3390/ma10030273 www.mdpi.com/journal/materials

http://www.mdpi.com/journal/materials http://www.mdpi.com http://www.mdpi.com/journal/materials

Materials 2017, 10, 273 2 of 12

to lattice mismatch and charge transfer due to chemical heterogeneity between the Fe oxide film and steel are unavoidable. There could be different factors, such as epitaxial strain, structural deformation, molecular orbital hybridization, and interfacial charge transfer, which affect the properties of the film. However, experimental and theoretical analyses suggest strain and charge transfer are two important extrinsic factors to alter the intrinsic properties of ultrathin Fe oxide films grown on a stainless steel (SS). In fact, strain and interfacial engineering have now become a common strategy to tailor a wide range of thin film properties, from crystalline structure [14], growth morphology (especially nanoscale assembly) [15], electronic band structure [16], magnetism [17], and carrier mobility [18] to superconductivity [19].

It is generally known that SS resistance to stress corrosion cracking is poor, which is largely affected by the structure, thickness, and composition of the passive film [20]. The strain is an effective approach to modulate the surface work function. Based on experimental observations and theoretical studies, we know that the work function is closely related to the corrosion potential, the lower work function of material, the lower corrosion potential is and the easier corrosion becomes, i.e., the work function is a sensitive parameter to the corrosion behavior [21]. Strain is expected to affect the fundamental properties of systems, and conversely can be used as an effective mean to tailor the properties of materials for potential applications.

From a theoretical point of view, the main interest in these compounds lies in the role of strong electronic correlations in determining their physical and chemical properties. Motivated by these recent experimental and theoretical studies, we have carried out a systematic study of the electronic properties of α-Fe2O3 film focusing on the effects of strain, based on first-principles calculations. We find that the band gap of the α-Fe2O3 film and work function can be tuned by strain. These calculation results allow us to conclude that the electronic structure and work function of α-Fe2O3 film could be modified by strain when the α-Fe2O3 film is grown on a SS, which can be very useful for explaining the effect of strain, future experimental studies as well as fundamentally understand the corrosion behavior.

2. Methods

First, as is typical for transition-metal compounds, both GGA and the LDA+U corrections reduce the LDA overbinding problem and increase the equilibrium volume which becomes close to the experimental value. Rohrbach et al. [22] performed a GGA+U calculation for Cr2O3 and obtained more reasonable results for the band structure. However, this approach is inaccurate for structural and magnetic properties. Mosey et al. [23] obtained better overall agreement with experiment for structural and spectral properties using the spherically averaged LSDA+U method with U − J = 3.2 eV. For α-Fe2O3, because Fe d bands are strongly correlated, researchers adopted the LSDA+U approach [24,25]. Therefore, we tend to use LDA+U method for α-Fe2O3 system. The hexagonal lattice of α-Fe2O3 film is shown in Figure 1a. The electronic band structures and electronic properties were calculated as before [26–30] in the framework of the (Slater exchange [31] plus Vosko–Wilk–Nusair correlation [32]) local density approximation LDA+U using Vienna Ab initio Simulation Package (VASP) package. The energy cutoff of 400 eV was selected to converge the total energy within 1 meV/atom on 5 × 5 × 5 and 5 × 5 × 1 (or 9 × 9 × 1) Monkhorst–Pack k-point mesh for bulk and film, respectively. For the calculation of band structures within the L(S)DA+U approach, it is hence strictly required to increase LMAXMIX (a parameter in VASP code) to 4 (d elements). For structural relaxation, all the atoms are allowed to relax until atomic forces are smaller than 0.01 eV/Å. The optimized lattice constant for bulk is a = 4.916 Å which is close to experimentally derived structural parameter 5.035 Å [33]. It is expected that different surface Fe and O terminations will also lead to significant differences in the electronic and work function of the systems. We defined the strain percent as (a − a0)/a0, where a0 is the experimental lattice constant without strain, and a is the lattice constant under compressive or tensile strain. The polar (0001) surface has been modeled by symmetric slabs containing 1–3 hexagonal unit cell layers for the Fe and O terminated surfaces and a 1 × 1 periodicity in the surface, containing 30 (33) to 90 (93) atoms, respectively. The use of symmetric slabs cancels

Materials 2017, 10, 273 3 of 12

out dipole moments, which can occur in nonsymmetric slabs. The vacuum layer is 15 Å thick for α-Fe2O3 films with strains up to ±6% (+ for tensile strain, − for compressive strain). The band gaps are calculated for different U parameters. The Coulomb repulsion is characterized by a spherically averaged Hubbard parameter U and a parameter J representing the screened exchange energy. While U depends on the spatial extension of the wave functions and on screening, J is an approximation of the Stoner exchange parameter and almost constant J ~1 eV. In our calculation the J is set to be 0.5 eV. Figure 1b shows the band gap of α-Fe2O3 bulk as a function of U parameter of Coulomb repulsion. The band gap increases with increasing U parameter. It is important to be aware of the fact that when using the LDA+U, in general, the total energy will depend on the parameters U and J. Thus, it is not meaningful to compare the total energies resulting from calculations with different U and/or J (U − J in the case of Dudarev’s approach [24]). The energy depends on the difference (U − J) introduced by Dudarev.

ELSDA+U = ELSDA + (U − J)

2 ∑σ

[( ∑ m1

nσm1,m1

) − (

∑ m1,m2

n̂σm1,m2 n̂ σ m2,m1

)] (1)

In Dudarev’s approach, the parameters U and J are not entered separately, only the difference (U − J) is meaningful. The more the Ueff